ADDRESS:Fenlukou Town Yu'an District Lu'an City Anhui China-237143
When refractory materials are used in glass kiln, they will be seriously damaged due to high temperature, flame, powder, atmosphere, air flow and liquid flow, which greatly affects the service life of the kiln. From the kiln, the use of refractory materials in the kiln begins, and improper operation will also cause large, even severe damage to the refractory material, which requires special attention. The following describes several types of damage.
The kiln powder, glass liquid and flame gas will erode the refractory material at high temperatures.
The erosion effect of the powder on the refractory material is mainly manifested in the erosion of the refractory by the alkaline vapor evaporated by the high temperature of the powder, such as the erosion of the surface of the silica brick, the internal "rat hole", etc., and the anti-pegal petrochemical in the checker brick. Function and so on. Furthermore, the ultrafine powder in the powder accumulates in the lattice of the regenerator to form a tumor, which blocks the lattice hole. In severe cases, the lattice brick collapses and is damaged, and is forced to be repaired. The erosion effect is exacerbated by the increase in temperature, and the increase in the melting temperature by 50 to 60 ° C shortens the service life by about one year. The front face wall, the feeding port, the front space of the melting section, the pool wall, the small furnace, the upper lattice of the regenerator, and the like are all damaged by the powder.
The corrosion effect of the glass liquid on the refractory material is much smaller than that of the powder, and the phase reaction between the glass liquid and the refractory interface layer is complicated. The glass solution first dissolves the free SiO2 in the refractory. The dissolution rate of mullite is small, and it accumulates at the interface between the glass liquid and the refractory material. Although the small crystal mullite is dissolved, the large crystal mullite even grows when used. After the refractory material is eroded, the composition in contact with it adds SiO2 and Al2O3 components. The melt will diffuse into the rest of the glass. During the diffusion process, the composition of the melt changes, the SiO2 and the lye increase, and the aggregation of the β-Al2O3 crystal occurs at the interface. Therefore, on the contact surface between the refractory and the glass, the first is Molai. The stone layer is followed by a layer of β-Al 2 O 3 followed by an unetched refractory material. After the refractory material is dissolved, the viscosity of the glass liquid is increased, which promotes the formation of a protective layer which is difficult to move on the surface of the refractory material, thereby weakening the effect of continuing erosion.
The erosive effect of molten glass on refractory materials depends on physical properties such as viscosity and surface tension. A glass with a low viscosity and a small surface tension is most likely to infiltrate the refractory material and is sucked into the interior from the pores of the surface, so that the entire refractory material is strongly eroded. High alkali glass has a low viscosity, and borosilicate glass has a small surface tension, so that its erosion is severe. Increasing the melting temperature reduces the viscosity and surface tension of the molten glass, which also accelerates the erosion. The glass liquid containing boric acid, phosphoric acid, fluorine, aluminum and antimony compound has a strong erosive effect on the refractory material, and strong convection of the molten glass and unstable liquid surface will wash away the protective layer and accelerate the erosion. For the refractory itself, the degree of corrosion is mainly related to its chemical composition, mineral composition and structural state. Uneven surface and crack of refractory material will intensify the erosion. The brick wall and pool wall brick joint at the liquid level are in the place where the glass liquid is easily damaged. The horizontal seam is more serious than the vertical seam, so the masonry surface is required. Smooth, small joints, and must be built in one piece.
Combustion products of gas and heavy oil (containing corrosive gases such as so2 and V2O5) and volatiles of individual batch components may also corrode refractory materials in flame spaces, furnaces, regenerators, etc. Different building materials will react with each other at high temperatures, resulting in damage. For example, 1600~1650 °C, clay bricks and silica bricks will react violently, high alumina bricks and silica bricks will have moderate reaction, and fused zirconium corundum bricks and silica bricks will react violently and be severely eutectic. The fused zirconium corundum brick reacts moderately with quartz brick and white foam, but reacts with the corundum brick. Therefore, corundum bricks can be used as transition materials.
The lattice used in the regenerator is also destroyed by the action of redox atmosphere. The damage mechanism mainly lies in the fact that the valence ions have different valence states in the oxidized and reduced states, and the coordination state is different, resulting in volume change, resulting in a decrease in product strength and cracking.
Under the action of high temperature for a long time, the refractory material will be melted (also called burned) or softened and damaged. Part of the kiln is partially overheated or the refractory material is not sufficiently refractory, and the refractory material is melted. Sometimes, the refractoriness is acceptable, but the load softening temperature is low. When used for a long time, the refractory material will soften and deform, which affects the stability and service life of the entire masonry. The severity of burnout depends on the temperature and the nature of the refractory material. The small furnace blasting port, the small furnace legs, the tongue, the regenerator chamber, the melting kiln and the chest wall are easily burnt parts.
3, crack damage
The cracking mainly occurs in the kiln stage. When the kiln is baked, a certain temperature difference occurs inside the refractory brick, and corresponding mechanical stress is generated. If the heating rate is too fast and exceeds the limit strength allowed by the refractory, cracks may occur and even break into pieces. The fused, highly sintered dense refractory material is the most susceptible to breakage. In addition to the stress generated by the temperature difference, the expansion or contraction caused by the change in the crystal form of the refractory material also causes stress. When the temperature rises too fast, the crystal form changes rapidly, the volume changes too much, and the stress is too large, causing the refractory material to crack. Therefore, in the kiln, the temperature of the kiln must be raised according to the pre-established kiln curve. After the kiln is kiln, the refractory material is exposed to high temperature for a long time, and the mechanical strength of the refractory material at the working temperature is much lower than that at room temperature. If the mechanical load acting on the refractory material is too large, the refractory material will be inelastically deformed (similar to the extremely viscous liquid flow), causing damage.
4, wear and tear
The glass liquid has the effect of dripping water and stone when flowing along the refractory material, and the refractory material is ground out of a groove, which is mechanical wear. The main wear site is at the glass level. In addition, it is also clearly visible at the flow of the circulating fluid (especially where the flow is disordered). Wear is exacerbated when liquid level fluctuations and liquid flow changes (such as those affected by temperature fluctuations).
Please send us your requirement by email.
Copyright © Greenergy Refractory and Insulation Material Co.,Ltd All Rights Reserved.